The Basic Copper Carbonate (WSDTY) top base glaze has just enough melt fluidity to produce a brilliant transparent (without colorant additions). However it does not have enough fluidity to pass the bubbles and heal over from the decomposition of this added copper carbonate! Why is lower glaze passing the bubbles? How can it melt better yet have 65% less boron? How can it not be crazing when the COE calculates to 7.7 (vs. 6.4)? First, it has 40% less Al2O3 and SiO2 (which normally stiffen the melt). Second, it has higher flux content that is more diversified. That zinc is a key to why it is melting so well and why it starts melting later (enabling unimpeded gas escape until then). It also benefits from the mixed-oxide-effect, the diversity itself improves the melt. And the crazing? The ZnO obviously pushes the COE down disproportionately to its percentage.
Wujiang Weishida Copper Technology Co.,Ltd. has 12,000 square meters of production base. By virtue of their sincere cooperation, reciprocity of the business philosophy for the industry users around the country to provide high-quality non-ferrous metal products. Weishida specializes in producing cuprous chloride, basic copper carbonate, copper acetate, copper oxide, copper sulfate. Our company has established a perfect quality assurance system, quality inspection and testing equipment, testing, testing and technology development strength, to ensure the stability of product quality, fully able to meet the pre-market after-sales service to provide users with the need.
Click Copper Chloride Dihydrate to learn about more information